2Plastic ProductsPlastics can be shaped into a wide variety of products:Molded partsExtruded sectionsFilmsSheetsInsulation coatings on electrical wiresFibers for textiles
3More Plastic ProductsIn addition, plastics are often the principal ingredient in other materials, such asPaints and varnishesAdhesivesVarious polymer matrix compositesMany plastic shaping processes can be adapted to produce items made of rubbers and polymer matrix composites
4Trends in Polymer Processing Applications of plastics have increased at a much faster rate than either metals or ceramics during the last 50 yearsMany parts previously made of metals are now being made of plasticsPlastic containers have been largely substituted for glass bottles and jarsTotal volume of polymers (plastics and rubbers) now exceeds that of metals
5Plastic Shaping Processes are Important Almost unlimited variety of part geometriesPlastic molding is a net shape processFurther shaping is not neededLess energy is required than for metals due to much lower processing temperaturesHandling of product is simplified during production because of lower temperaturesPainting or plating is usually not required
6Two Types of Plastics 1. Thermoplastics Thermosets Chemical structure remains unchanged during heating and shapingMore important commercially, comprising more than 70% of total plastics tonnageThermosetsUndergo a curing process during heating and shaping, causing a permanent change (cross‑linking) in molecular structureOnce cured, they cannot be remelted
7Polymer MeltsTo shape a thermoplastic polymer it must be heated so that it softens to the consistency of a liquidIn this form, it is called a polymer meltImportant properties of polymer melts:ViscosityViscoelasticity
8Viscosity of Polymer Melts Fluid property that relates shear stress to shear rate during flowDue to its high molecular weight, a polymer melt is a thick fluid with high viscosityMost polymer shaping processes involve flow through small channels or die openingsFlow rates are often large, leading to high shear rates and shear stresses, so significant pressures are required to accomplish the processes
9Viscosity and Shear Rate Viscosity of a polymer melt decreases with shear rate, thus the fluid becomes thinner at higher shear ratesFigure Viscosity relationships for Newtonian fluid and typical polymer melt.
10Viscosity and Temperature Viscosity decreases with temperature, thus the fluid becomes thinner at higher temperaturesFigure Viscosity as a function of temperature for selected polymers at a shear rate of 103 s-1.
11Viscoelasticity Combination of viscosity and elasticity Die SwellCombination of viscosity and elasticityPossessed by both polymer solids and polymer meltsExample: die swell in extrusion, in which the hot plastic expands when exiting the die openingExtruded polymer "remembers" its previous shape when in the larger cross section of the extruder, tries to return to it after leaving the die orifice
12ExtrusionCompression process in which material is forced to flow through a die orifice to provide long continuous product whose cross‑sectional shape is determined by the shape of the orificeWidely used for thermoplastics and elastomers to mass produce items such as tubing, pipes, hose, structural shapes, sheet and film, continuous filaments, and coated electrical wireCarried out as a continuous process; extrudate is then cut into desired lengths
13ExtruderFigure Components and features of a (single‑screw) extruder for plastics and elastomersMajor components: Barrel, ScrewDie - not an extruder component (Special tool that must be fabricated for particular profile to be produced )
14Extruder BarrelInternal diameter typically ranges from 25 to 150 mm (1.0 to 6.0 in.)L/D ratios usually between 10 and 30: higher ratios for thermoplastics, lower ratios for elastomersFeedstock fed by gravity onto screw whose rotation moves material through barrelElectric heaters melt feedstock; subsequent mixing and mechanical working adds heat which maintains the melt
15Extruder Screw Divided into sections to serve several functions: Feed section - feedstock is moved from hopper and preheatedCompression section - polymer is transformed into fluid, air mixed with pellets is extracted from melt, and material is compressedMetering section - melt is homogenized and sufficient pressure developed to pump it through die opening
16Extruder ScrewFigure Details of an extruder screw inside the barrel.
17Melt Flow in ExtruderAs screw rotates inside barrel, polymer melt is forced to move forward toward die; as in an Archimedian screwPrincipal transport mechanism is drag flow, Qd, resulting from friction between the viscous liquid and the rotating screwCompressing the polymer melt through the die creates a back pressure that reduces drag flow transport (called back pressure flow, Qb )Resulting flow in extruder is Qx = Qd – Qb
18Die End of ExtruderProgress of polymer melt through barrel leads ultimately to the die zoneBefore reaching die, the melt passes through a screen pack - series of wire meshes supported by a stiff plate containing small axial holesFunctions of screen pack:Filter out contaminants and hard lumpsBuild pressure in metering sectionStraighten flow of polymer melt and remove its "memory" of circular motion from screwThe shape of the die orifice determines the cross‑sectional shape of the extrudateCommon die profiles and corresponding extruded shapes:Solid profilesHollow profiles, such as tubesWire and cable coatingSheet and filmFilamentsStructural shapesDoor and window moldingsAutomobile trimHouse siding
19Extrusion Die for Solid Cross Section Figure (a) Side view cross‑section of an extrusion die for solid regular shapes, such as round stock; (b) front view of die, with profile of extrudate. Die swell is evident in both views.
20Hollow ProfilesExamples: tubes, pipes, hoses, and other cross‑sections containing holesHollow profiles require mandrel to form the shapeMandrel held in place using a spiderPolymer melt flows around legs supporting the mandrel to reunite into a monolithic tube wallMandrel often includes an air channel through which air is blown to maintain hollow form of extrudate during hardening
21Extrusion Die for Hollow Shapes Figure Side view cross‑section of extrusion die for shaping hollow cross‑sections such as tubes and pipes; Section A‑A is a front view cross‑section showing how the mandrel is held in place; Section B‑B shows the tubular cross‑section just prior to exiting the die; die swell causes an enlargement of the diameter.
22Wire and Cable CoatingPolymer melt is applied to bare wire as it is pulled at high speed through a dieA slight vacuum is drawn between wire and polymer to promote adhesion of coatingWire provides rigidity during cooling - usually aided by passing coated wire through a water troughProduct is wound onto large spools at speeds up to 50 m/s (10,000 ft/min)
23Extrusion Die for Coating Wire Figure Side view cross‑section of die for coating of electrical wire by extrusion.
24Polymer Sheet and Film Film - thickness below 0.5 mm (0.020 in.) Packaging - product wrapping material, grocery bags, and garbage bagsStock for photographic filmPool covers and liners for irrigation ditchesSheet - thickness from 0.5 mm (0.020 in.) to about 12.5 mm (0.5 in.)Flat window glazingThermoforming stock
25Materials and Processes for Polymer Sheet and Film All thermoplastic polymersPolyethylene, mostly low density PEPolypropylenePolyvinylchlorideCellophaneMost widely used processes are continuous, high production operationsProcesses include:Slit‑Die Extrusion of Sheet and FilmBlown‑Film Extrusion ProcessCalendering
26Slit‑Die Extrusion of Sheet and Film Production of sheet and film by conventional extrusion, using a narrow slit as the die openingSlit may be up to 3 m (10 ft) wide and as narrow as around 0.4 mm (0.015 in)A problem is uniformity of thickness throughout width of stock, due to drastic shape change of polymer melt as it flows through dieEdges of film usually must be trimmed because of thickening at edges
27Slit Die ExtrusionFigure One of several die configurations for extruding sheet and film.
28Blown‑Film Extrusion Process Combines extrusion and blowing to produce a tube of thin filmProcess sequence:Extrusion of tubeTube is drawn upward while still molten and simultaneously expanded by air inflated into it through dieAir is blown into tube to maintain uniform film thickness and tube diameter
29Blown-film ProcessFigure Blown‑film process for high production of thin tubular film.
30CalenderingFeedstock is passed through a series of rolls to reduce thickness to desired gageExpensive equipment, high production ratesProcess is noted for good surface finish and high gage accuracyTypical materials: rubber or rubbery thermoplastics such as plasticized PVCProducts: PVC floor covering, shower curtains, vinyl table cloths, pool liners, and inflatable boats and toys
31Figure 13.17 A typical roll configuration in calendering
32Injection MoldingPolymer is heated to a highly plastic state and forced to flow under high pressure into a mold cavity where it solidifies and the molding is then removed from cavityProduces discrete components almost always to net shapeTypical cycle time 10 to 30 sec, but cycles of one minute or more are not uncommonMold may contain multiple cavities, so multiple moldings are produced each cycle
33Injection Molded Parts Complex and intricate shapes are possibleShape limitations:Capability to fabricate a mold whose cavity is the same geometry as partShape must allow for part removal from moldPart size from 50 g (2 oz) up to 25 kg (more than 50 lb), e.g., automobile bumpersInjection molding is economical only for large production quantities due to high cost of mold
34Polymers for Injection Molding Injection molding is the most widely used molding process for thermoplasticsSome thermosets and elastomers are injection moldedModifications in equipment and operating parameters must be made to avoid premature cross‑linking of these materials before injection
35Injection Molding Machine Two principal components:Injection unitMelts and delivers polymer meltOperates much like an extruderClamping unitOpens and closes mold each injection cycle
37Injection Molding Machine Figure Diagram of an injection molding machine, reciprocating screw type (some mechanical details are simplified).
38Injection Unit of Molding Machine Consists of barrel fed from one end by a hopper containing supply of plastic pelletsInside the barrel is a screw which:Rotates for mixing and heating polymerActs as a ram (i.e., plunger) to inject molten plastic into moldNon‑return valve near tip of screw prevents melt flowing backward along screw threadsLater in molding cycle ram retracts to its former position
39Clamping Unit of Molding Machine Functions:Holds two halves of mold in proper alignment with each otherKeeps mold closed during injection by applying a clamping force sufficient to resist injection forceOpens and closes mold at the appropriate times in molding cycle
40Injection Molding Cycle Figure Typical molding cycle: (2) melt is injected into cavity.Figure Typical molding cycle: (1) mold is closed
41Injection Molding Cycle Figure Typical molding cycle: (4) mold opens and part is ejected.Figure Typical molding cycle: (3) screw is retracted.
42The Mold The special tool in injection molding Custom‑designed and fabricated for the part to be producedWhen production run is finished, the mold is replaced with a new mold for the next partVarious types of mold for injection molding:Two-plate moldThree-plate moldHot-runner mold
43Two-Plate MoldFigure Details of a two‑plate mold for thermoplastic injection molding: (a) closed. Mold has two cavities to produce two cup‑shaped parts with each injection shot.
44Two-Plate MoldFigure Details of a two‑plate mold for thermoplastic injection molding: (b) open
45Two‑Plate Mold Features Cavity – geometry of part but slightly oversized to allow for shrinkageCreated by machining of mating surfaces of two mold halvesDistribution channel through which polymer melt flows from nozzle into mold cavitySprue - leads from nozzle into moldRunners - lead from sprue to cavity (or cavities)Gates - constrict flow of plastic into cavity
46More Two‑Plate Mold Features Ejection system – to eject molded part from cavity at end of molding cycleEjector pins built into moving half of mold usually accomplish this functionCooling system - consists of external pump connected to passageways in mold, through which water is circulated to remove heat from the hot plasticAir vents – to permit evacuation of air from cavity as polymer melt rushes in
47Three‑Plate MoldUses three plates to separate parts from sprue and runner when mold opensAdvantages over two-plate mold:As mold opens, runner and parts disconnect and drop into two containers under moldAllows automatic operation of molding machine
48Hot‑Runner MoldEliminates solidification of sprue and runner by locating heaters around the corresponding runner channelsWhile plastic in mold cavity solidifies, material in sprue and runner channels remains molten, ready to be injected into cavity in next cycleAdvantage:Saves material that otherwise would be scrap in the unit operation
49Injection Molding Machines Injection molding machines differ in both injection unit and clamping unitName of injection molding machine is based on the type of injection unit usedReciprocating-screw injection molding machinePlunger-type injection molding machineSeveral clamping designsMechanical (toggle)Hydraulic
50ShrinkageReduction in linear size during cooling from molding to room temperaturePolymers have high thermal expansion coefficients, so significant shrinkage occurs during solidification and cooling in moldTypical shrinkage values:Plastic Shrinkage, mm/mm (in/in)Nylon‑6,PolyethylenePolystyrenePVC
51Compensation for Shrinkage Dimensions of mold cavity must be larger than specified part dimensions:Dc = Dp + DpS + DpS2where Dc = dimension of cavity; Dp = molded part dimension, and S = shrinkage valueThird term on right hand side corrects for shrinkage in the shrinkage
52Shrinkage Factors Fillers in the plastic tend to reduce shrinkage Injection pressure – higher pressures force more material into mold cavity to reduce shrinkageCompaction time - similar effect – longer time forces more material into cavity to reduce shrinkageMolding temperature - higher temperatures lower polymer melt viscosity, allowing more material to be packed into mold to reduce shrinkage
53Compression MoldingA widely used molding process for thermosetting plasticsAlso used for rubber tires and polymer matrix composite partsMolding compound available in several forms: powders or pellets, liquid, or preformAmount of charge must be precisely controlled to obtain repeatable consistency in the molded product
54Compression MoldingFigure Compression molding for thermosetting plastics: (1) charge is loaded, (2) and (3) charge is compressed and cured, and (4) part is ejected and removed.
55Molds & Materials for Compression Molding Simpler than injection moldsNo sprue and runner system in a compression moldProcess itself generally limited to simpler part geometries due to lower flow capabilities of TS materialsMold must be heated, usually by electric resistance, steam, or hot oil circulationMolding materials:Phenolics, melamine, urea‑formaldehyde, epoxies, urethanes, and elastomersTypical compression-molded products:Electric plugs, sockets, and housings; pot handles, and dinnerware plates
56Pot Transfer MoldingFigure (a) Pot transfer molding: (1) charge is loaded into pot, (2) softened polymer is pressed into mold cavity and cured, and (3) part is ejected.
57Plunger Transfer Molding Figure (b) plunger transfer molding: (1) charge is loaded into pot, (2) softened polymer is pressed into mold cavity and cured, and (3) part is ejected.
58Compression vs. Transfer Molding In both processes, scrap is produced each cycle as leftover material, called the cullThe TS scrap cannot be recoveredTransfer molding is capable of molding more intricate part shapes than compression molding but not as intricate as injection moldingTransfer molding lends itself to molding with inserts, in which a metal or ceramic insert is placed into cavity prior to injection, and the plastic bonds to insert during molding
59Blow MoldingMolding process in which air pressure is used to inflate soft plastic into a mold cavityImportant for making one‑piece hollow plastic parts with thin walls, such as bottlesBecause these items are used for consumer beverages in mass markets, production is typically organized for very high quantities
60Blow Molding Process Accomplished in two steps: Fabrication of a starting tube, called a parisonInflation of the tube to desired final shapeForming the parison is accomplished by eitherExtrusion orInjection molding
61Extrusion Blow Molding Figure Extrusion blow molding: (1) extrusion of parison; (2) parison is pinched at the top and sealed at the bottom around a metal blow pin as the two halves of the mold come together; (3) the tube is inflated so that it takes the shape of the mold cavity; and (4) mold is opened to remove the solidified part.
62Injection Blow Molding Figure Injection blow molding: (1) parison is injected molded around a blowing rod; (2) injection mold is opened and parison is transferred to a blow mold; (3) soft polymer is inflated to conform to the blow mold; and (4) blow mold is opened and blown product is removed.
63Stretch Blow MoldingVariation of injection blow molding in which blowing rod stretches the soft parison for a more favorable stressing of polymer than conventional blow moldingResulting structure is more rigid, more transparent, and more impact resistantMost widely used material is polyethylene terephthalate (PET) which has very low permeability and is strengthened by stretch blow moldingCombination of properties makes it ideal as container for carbonated beverages
64Stretch Blow MoldingFigure Stretch blow molding: (1) injection molding of parison; (2) stretching; and (3) blowing.
65Materials and Products in Blow Molding Blow molding is limited to thermoplasticsMaterials: high density polyethylene, polypropylene (PP), polyvinylchloride (PVC), and polyethylene terephthalateProducts: disposable containers for beverages and other liquid consumer goods, large shipping drums (55 gallon) for liquids and powders, large storage tanks (2000 gallon), gasoline tanks, toys, and hulls for sail boards and small boats
66ThermoformingFlat thermoplastic sheet or film is heated and deformed into desired shape using a moldHeating usually accomplished by radiant electric heaters located on one or both sides of starting plastic sheet or filmWidely used in packaging of products and to fabricate large items such as bathtubs, contoured skylights, and internal door liners for refrigerators
67Vacuum ThermoformingFigure Vacuum thermoforming: (1) a flat plastic sheet is softened by heating, (2) the softened sheet is placed over a concave mold cavity, (3) a vacuum draws the sheet into the cavity, (4) plastic hardens on contact with the cold mold surface, and the part is removed and subsequently trimmed from the web.
68Materials for Thermoforming Only thermoplastics can be thermoformed,Extruded sheets of thermosetting or elastomeric polymers have already been cross‑linked and cannot be softened by reheatingCommon TP polymers: polystyrene, cellulose acetate, cellulose acetate butyrate, ABS, PVC, acrylic (polymethylmethacrylate), polyethylene, and polypropylene